mineralogical solutions for mineralogy, traditionally associated with concentrator studies, is ......
Post on 18-Jun-2020
Embed Size (px)
T r a n s a c t i o n
P a p e r
Mineralogy can be thought of as an extra dimension in metallurgical planning and investigations, especially when combined with chemical or metallurgical information. Strictly defined as the study of minerals, including their distribution, identification, physical properties, and chemical composition, mineralogy is traditionally associated with the geosciences and concentrator studies, but can equally be applied to problems encountered in metallurgy1,2.
The most basic technique used in mineralogy is optical microscopy; in addition, modern phase characterization relies on the measurement of crystal structure and orientation by means of techniques such as X- ray diffractometry (XRD) and electron- backscattered diffractometry (EBSD), and the determination of phase shape, size, modal abundance, and composition with electron- beam techniques such as scanning electron microscopy and electron-probe micro-analysis. A mineralogical assessment will usually rely on a combination of several techniques.
Mineralogical applications in pyro- metallurgy
Mineralogy can be used to characterize solid phases in furnace or roaster feeds and in the products of roasting, smelting, and converting. Some of the processes in which mineralogy can contribute are outlined below, and specific applications are described.
Knowledge of the phase-chemical compositions and structures of roaster feed and products, and their variations over time, allows processes to be designed. The benefit of this knowledge can be seen, for example, when evaluating the performance of the oxygen carrier in chemical-looping combustion (CLC).
Application: chemical-looping combustion
CLC is a technology being developed in labora- tories round the world. It addresses the matter of CO2 emissions to atmosphere by inherently separating the greenhouse gas during combustion3. A pure CO2 stream can be sequestrated. In a CLC process an oxygen carrier—an oxide, either natural or synthesized—is made to circulate between two fluidized-bed reactors, an ‘air reactor’ and a ‘fuel reactor’. Fuel (e.g. natural gas or coal) is introduced to the fuel reactor, where it reduces the oxygen carrier and forms CO2 and H2O
Mineralogical solutions for pyrometallurgical problems by L. Andrews* and P. den Hoed*
Mineralogy, traditionally associated with concentrator studies, is being increasingly applied to problems in pyrometallurgy. Such investigations commonly make use of a number of techniques, and the results are combined for a meaningful interpretation, which can lead to a successful solution for the problem.
Mineralogical techniques are described for various pyrometal- lurgical operations. Examples are given of studies and investi- gations involving mineralogy in chemical-looping combustion, feed monitoring to platinum-smelting furnaces, and losses to slag in base metal and platinum smelting.
Keywords mineralogy, phase-chemical, chemical-looping combustion, XRD, SEM, EDS, QEMSCAN, PGM, slag, matte, ilmenite.
* Anglo American Research, Johannesburg, South Africa.
© The Southern African Institute of Mining and Metallurgy, 2011. SA ISSN 0038–223X/3.00 + 0.00. This paper was first presented at the Southern African Pyrometallurgy Conference, 6–9 March 2011, Misty Hills, Muldersdrift.
675The Journal of The Southern African Institute of Mining and Metallurgy VOLUME 111 OCTOBER 2011 ▲
Mineralogical solutions for pyrometallurgical problems
(Equation  describes the reaction in schematic form). Condensation separates H2O from CO2. The reduced oxygen carrier is then transferred to the air reactor where, in contact with air diluted by nitrogen, it is re-oxidized (Equation )3. Temperatures in the two units run at about 950°C. Reaction 1 is often endothermic; reaction 2 is exothermic. Nevertheless, the total heat evolved from both reactions equals that released under normal combustion, where oxygen is in direct contact with the fuel. Thus, without losing energy, but achieving a separation of CO2 from N2, CLC has an emission advantage over normal combustion.
The matter that concerns us here, however, is the behaviour of the oxygen carrier. A first requirement is the selection of a good carrier. Carriers are required to exhibit high reactivity, good mechanical strength, and resistance to attrition and agglomeration. The carrier particles should also retain their integrity during many cycles of oxidation and reduction. Candidates have included oxides of iron, manganese, cobalt, nickel, and copper4,5. Ilmenite (FeTiO3) has become a popular oxygen carrier, because it is abundant and comparatively cheap. It has been tested for a number of years, now, but it has never been fully examined; its effectiveness has been determined by such measures as how much fuel it can convert and how quickly and, in doing so, what its oxygen-carrying capacity is. That is not to say that there have not been reports characterizing the oxygen carrier: phases have been identified, but their distribution in particles has not been examined. In recent years studies have
published images of the internal structures of particles, but these have not been tied to the distribution of phases. Some of the images nevertheless point to the performance of the oxygen carrier over the long term. So, for example, ‘ilmenite’ particles after a number of cycles show an iron-enriched (oxide) rim on the surface of particles and an exfoliation shell6. The shell appears somewhat fragile; it is very likely that the mechanical forces in a fluidized bed will, in time, break this shell from the rest of the particle. Each subsequent shell will, in all likelihood, meet the same fate. This possibility warrants investigating.
The changes that iron-titanium oxides undergo during redox cycles in CLC can be evaluated in an informative manner by referring to the chemical thermodynamics of the oxide system. A useful tool in this regard is the equilibrium phase diagram, which is well documented for the Fe-Ti-O system. The phases and their relations described by the diagram can be compared with those observed in samples of actual oxygen carriers at different stages in the process. Using XRD, and by examining (polished) sections of particles under the electron microscope and measuring phase compositions with energy-dispersive X-ray spectroscopy (EDS), one can determine phase-chemical compositions in the samples and compare them with those described in the appropriate phase diagrams. A first step in this direction has been made with the application of phase relations in the system Fe-Ti-O to the performance of ‘ilmenite’ in CLC7. The chemical thermodynamics predict that FeTiO3 oxidizes to Fe2TiO5 (pseudobrookite) and TiO2 (rutile), a condition reflected by a move on the oxygen reaction line XY towards Y (see Figure 1). Subsequent reduction returns the oxide either to FeTiO3 (ilmenite) if the system is held at equilibrium or to Fe2TiO4 (ulvöspinel) if conditions prevent TiO2 (rutile) from taking part in the reduction. Which of the oxides actually
676 OCTOBER 2011 VOLUME 111 The Journal of The Southern African Institute of Mining and Metallurgy
Figure 1—Phase relations in the system Fe-Fe2O3-TiO2-Ti2O3 at 1000°C8
forms, how much of it forms, and how it is distributed has yet to be confirmed. Once we know this, a comparison of predicted and observed outcomes will allow us to evaluate an aspect of the performance of the oxygen carrier: how close to the limit (where metallic iron is formed—an undesirable outcome) the oxygen carrier can be pushed in the fuel reactor, and therefore the extent to which the oxygen transport capacity of the carrier is diminished (if at all).
The oxygen transport capacity is defined as
where mox is the mass of a carrier in its oxidized state and mred is its mass in the reduced state. The higher the oxygen transport capacity, the less the oxygen carrier required for the job. The oxygen transport capacity of FeTiO3 (ilmenite) is 5.0%, which compares with 21.4% for Ni-NiO and 20.1% for Cu-CuO. If TiO2 (rutile), once formed, remains inert in subsequent cycles, then one can improve the oxygen transport capacity for iron-titanium oxides only slightly by synthesizing either Fe2TiO5 (pseudobrookite) or Fe2TiO4 (ulvöspinel). Ro rises to 6.7%, which remains a compara- tively low value. Any diminished capacity, by not reducing or oxidizing the carrier to its full extent, only makes matters worse. Confirmation of the phases formed, their individual compositions, and distributions throughout the carrier particles will help identify the nature of any diminished capacity. It will provide an important piece in the puzzle and do much to establish the full potential of ilmenite as an oxygen carrier in chemical-looping combustion.
Several types of furnace feed (ore concentrates or flash-dryer products) may possess very similar chemical compositions, but display completely different melting characteristics. Accurate knowledge of the mineral content allows prediction of the energy requirements, the melting temperature, and the matte fall.
Application (furnace feed)
Concentrates (smelter feeds) produced from the Bushveld Complex in North West and Limpopo provinces by Anglo Platinum Ltd are routinely monitored by means of mineralogical and chemical analysis. Merensky Reef, UG-2, and Platreef final concentrates are sampled at the concen- trators; flash-dryer feeds are sampled at the smelters9. Automated mineralogy techniq